**5.7 ** **Discussion of the Crystal Field Parameters**

**The problem is to parameterize the four strong bands observed**
**in the experiment at 19000, 15800, 13500 and 6000 cm ^ .** **The results of**

2 8

**a d ’ ** **cubic field calculation are reproduced in Figure 5.1 from**

**reference [11]. For the present case spin-orbit, B, and C have not been**
**used as entirely free parameters, rather they have been given values**

2+
**slightly lower than the free ion values for Ni**

**Calculation of selection rules for C„ ** **3Ä2** **3Ä2 and 3A2** **3E**
**3v**

**electric dipole transitions have been made using the coupling coefficients of**
**Koster [12](see Appendix I ) . The results are summarised for the infra-red band in**
**Figure 5.2. It means that a 3A2 -*■ 3A£ will only give one strong tt transition from**

**the T3 component of the ground state (the Greek script denotes the**
**spin-orbit component of the trigonal term).** **This is the observed**

**situation for the 13500 cm ^ band and consequently the line is assigned**
**to ^** **2(^3) -> 3A2( E 3) transition.**

**B = 610** **cm-1** **C = 2500 cm ^** **v = 800 cm**
**C = 155** **cm-1**

**The calculation also suggests that transitions from the ****T****3**
**component of the ground state should give three lines with the symmetry**
**of the excited state being T^, T2 and T3 belonging to a 3E trigonal level.**

**This is exactly what is observed in the 6000 cm ^ band. ** **Furthermore,**

**the hot band possibly to an ****T****3 level is also produced in the model. ** **So**

**the components of the spin-orbit split °E are all located.**

**With the above assignments it is possible to select two values**
**of Dq, about -600 cm ^ and -320 cm \ which give rise to spin-allowed**

**bands at 6000 and 13500 cm \ ** **In the first model (A) they would arise**

**from trigonally split components of the dTi term, whereas in the second**
**model (B) the infra-red band arises from this term and the strong bands**

**o b**

**in the visible would have their origin in the Tj term.**

**There are, however, a number of indications that model B with**
**the lower cubic field parameter is actually the correct physical**

**situation. The splitting of the 3T t e r m into the 3E and 3Ä trigonal**

**components varies as ~(v-v') and that of the 3T^a as ~(v+vT). ** **To achieve**

**the observed energy level ordering with model A requires a large negative**

**v and positive v ’.** **However, such parameter values do not give the T3**

**component of JA2 as the ground state. ** **Model B with a positive v gives**

**the correct order of ground state components and increasing the magnitude**

**of —v f reduces the ground state splitting. ** **In addition, this model gives**

**the right ordering of the excited states.**

**The A level (at 15800 cm ** **giving the rather weak band at**

**15800 cm ^ is not predicted, however, and is an outstanding difficulty,**
**and remained so even when attempting to adjust the crystal field parameters**
**in both minor and major ways (see Appendix II). We have not been able**
**in any of these attempts to obtain a triplet level (S = 1) at this position**
**while simultaneously fitting the other stronger bands (20000, 13500 and**

75,000

I 5,000

10,000

**Figure 5.1. ** **Energy level curves for a d 8 electronic system immersed in**

**a field of octahedral symmetry for c = - 550 cm"1 , B = 950 cm"1 and**
**C = 3150 cm"1 [11].**

**r 3** _{r 3 s+ }

_{> ,|r}_{'}_{3}

_{> ,|r}

**4 3 s 0 >Ir 3 s 0 >**

_{s_ >}**Toll’s s+ > + -^lr3**

*T I*

**^ 3 S+****" T ^ S**

**|r**2** s+ > , | r**2

**S >**

**lr2 SO >**

**(not observed)**Ir2 s0 > lr2 s+ >>l s. >

**s**

**s**

### >

### >

**Figure** **5.2. ** **The selection rules for the infra-red band allowed**

**O A**

**transitions are indicated. ** **All of the ** **spin-orbit components**
**are observed. ** **The 'hot' line at 6408 cm ^ is not observed at**
**low temperatures because it violates the spin-conservation rule**
**(Am^ =0). ** **The line observed at 4317 cm ^ might be due to the**
3**A**2( r 3 ) **-*• **

### 3**A**2**(r3) **

**transition.**

**The spin-orbit functions are**

**composed from the table of coupling coefficients in Appendix I.**

**6000) as triplets, i.e. spin allowed. ** **The strength of the 15800 cm ^**
**indicates that it is more likely anyway to arise from a singlet level**

**and hence to be associated with a spin-forbidden transition. ** **Familiarity**

**. **2**+**

**with Ni ** **spin-forbidden transitions in other systems would suggest that**

**this could arise from *E or the 1T2-** **However, of these the only T****\**** or**
**T2 level is that associated with the 1T2* This state is split in**

o **b**

**similar fashion (order and magnitude) to the higher ^Tj ** **band and hence**

**q * ** **O ** **b ** **• ** **•**

**always appears below the A2 component of the Tj ** **which is claimed**

**to lie at 13500 cm ** **.** **The spin-orbit splitting of the 3Ä2 itself, even**

**allowing for the interaction with this state, cannot displace by**

**1 ** O **A**

**2300 cm ** **from the '3A2(r'3) component (see Fig. 5.3). ** **Further experiments**

**such as EPR/MCD double resonance seem desirable to conclusively establish**
**that this band does indeed arise from the same centre.**

**An energy level diagram based on model B is shown in Figure 5.2**
**where D q , B, C and £ are fixed and the trigonal field components are**

**v ’** **1**

**varied in a fixed ratio — = - — and we see that the spin-allowed bands**

**are reasonably well predicted. ** **It will be shown in the next section**

**(Part B) that a similar value of Dq is used to fit the spectrum of**
**2+**

**E**

**N**

**E**

**R**

**G**

**Y**

**(**

**c**

**m**

*****rH

**I**